Successfully reported this slideshow.
Upcoming SlideShare
×

# Chapter 2 solutions

3,290 views

Published on

Shigley's Mechanical Engineering Design 9th Edition Solutions Manual

• Full Name
Comment goes here.

Are you sure you want to Yes No
• @koktonglim welcome boss

Are you sure you want to  Yes  No
• thx boss ~

Are you sure you want to  Yes  No

### Chapter 2 solutions

1. 1. Chapter 2 2-1 From Tables A-20, A-21, A-22, and A-24c, (a) UNS G10200 HR: S ut = 380 (55) MPa (kpsi), S yt = 210 (30) Mpa (kpsi) Ans. (b) SAE 1050 CD: S ut = 690 (100) MPa (kpsi), S yt = 580 (84) Mpa (kpsi) Ans. (c) AISI 1141 Q&T at 540C (1000F): S ut = 896 (130) MPa (kpsi), S yt = 765 (111) Mpa (kpsi) Ans. (d) 2024-T4: S ut = 446 (64.8) MPa (kpsi), S yt = 296 (43.0) Mpa (kpsi) Ans. (e) Ti-6Al-4V annealed: S ut = 900 (130) MPa (kpsi), S yt = 830 (120) Mpa (kpsi) Ans. ______________________________________________________________________________ 2-2 (a) Maximize yield strength: Q&T at 425C (800F) Ans. (b)Maximize elongation: Q&T at 650C (1200F) Ans. ______________________________________________________________________________ Conversion of kN/m3 to kg/ m3 multiply by 1(103) / 9.81 = 102 AISI 1018 CD steel: Tables A-20 and A-5 3 S y 370 10    47.4 kN  m/kg Ans.  76.5 102  2011-T6 aluminum: Tables A-22 and A-5 3 S y 169 10    62.3 kN  m/kg Ans.  26.6 102  Ti-6Al-4V titanium: Tables A-24c and A-5 830 103  Sy   187 kN  m/kg Ans.  43.4 102  ASTM No. 40 cast iron: Tables A-24a and A-5.Does not have a yield strength. Using the ultimate strength in tension 3 Sut 42.5  6.89  10    40.7 kN  m/kg Ans 70.6 102   ______________________________________________________________________________ 2-3 2-4 AISI 1018 CD steel: Table A-5 6 E 30.0 10    106 106  in Ans.  0.282 2011-T6 aluminum: Table A-5 6 E 10.4 10    106 106  in Ans. 0.098  Ti-6Al-6V titanium: Table A-5 Chapter 2 - Rev. D, Page 1/19
2. 2. E  16.5 106   103 106  in Ans. 0.160 No. 40 cast iron: Table A-5 6 E 14.5 10    55.8 106  in Ans. 0.260  ______________________________________________________________________________  2-5 2G (1  v)  E From Table A-5 Steel: v  Aluminum:  v 30.0  2 11.5  2 11.5  v Beryllium copper: E  2G 2G  0.304 Ans. 10.4  2  3.90  0.333 2  3.90 v 2  7.0   0.286 Ans. 14.5  2  6.0   0.208 Ans. 2  6.0  ______________________________________________________________________________ Gray cast iron: 2-6 v 18.0  2  7.0  Ans. (a) A 0 =  (0.503)2/4,  = P i / A 0 For data in elastic range,  =  l / l 0 =  l / 2 A l l  l0 l For data in plastic range,     1  0 1 l0 l0 l0 A On the next two pages, the data and plots are presented. Figure (a) shows the linear part of the curve from data points 1-7. Figure (b) shows data points 1-12. Figure (c) shows the complete range. Note: The exact value of A 0 is used without rounding off. (b) From Fig. (a) the slope of the line from a linear regression is E = 30.5 Mpsi Ans. From Fig. (b) the equation for the dotted offset line is found to be  = 30.5(106)  61 000 (1) The equation for the line between data points 8 and 9 is  = 7.60(105) + 42 900 (2) Chapter 2 - Rev. D, Page 2/19
3. 3. Solving Eqs. (1) and (2) simultaneously yields  = 45.6 kpsi which is the 0.2 percent offset yield strength. Thus, S y = 45.6 kpsi Ans. The ultimate strength from Figure (c) is S u = 85.6 kpsi Ans. The reduction in area is given by Eq. (2-12) is R A0  Af A0 100   0.1987  0.1077 100   45.8 % 0.1987 Pi 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 0 1000 2000 3000 4000 7000 8400 8800 9200 8800 9200 9100 13200 15200 17000 16400 14800   0 Data Point 0 0.0004 0.0006 0.001 0.0013 0.0023 0.0028 0.0036 0.0089 0.1984 0.1978 0.1963 0.1924 0.1875 0.1563 0.1307 0.1077 0.00020 0.00030 0.00050 0.00065 0.00115 0.00140 0.00180 0.00445 0.00158 0.00461 0.01229 0.03281 0.05980 0.27136 0.52037 0.84506 Ans. 0 5032 10065 15097 20130 35227 42272 44285 46298 44285 46298 45795 66428 76492 85551 82531 74479 l, A i (a) Linear range Chapter 2 - Rev. D, Page 3/19
4. 4. (b) Offset yield (c) Complete range (c) The material is ductile since there is a large amount of deformation beyond yield. (d) The closest material to the values of S y , S ut , and R is SAE 1045 HR with S y = 45 kpsi, S ut = 82 kpsi, and R = 40 %. Ans. ______________________________________________________________________________ 2-7 To plot  true vs., the following equations are applied to the data. P  true  A Eq. (2-4) Chapter 2 - Rev. D, Page 4/19
5. 5.   ln A0   (0.503)2 for 0  l  0.0028 in   ln where l l0 A0 A for l  0.0028 in  0.1987 in 2 4 The results are summarized in the table below and plotted on the next page. The last 5 points of data are used to plot log  vs log  The curve fit gives m = 0.2306 log  0 = 5.1852   0 = 153.2 kpsi Ans. For 20% cold work, Eq. (2-14) and Eq. (2-17) give, A = A 0 (1 – W) = 0.1987 (1 – 0.2) = 0.1590 in2 A0 0.1987  ln  0.2231 0.1590 A Eq. (2-18): S y   0 m  153.2(0.2231)0.2306  108.4 kpsi   ln Ans. Eq. (2-19), with Su  85.6 from Prob. 2-6,  Su  Su 85.6   107 kpsi 1  W 1  0.2 P L 0 1000 2000 3000 4000 7000 8400 8800 9200 9100 13200 15200 17000 16400 14800 0 0.0004 0.0006 0.001 0.0013 0.0023 0.0028 0.0036 0.0089 A 0.198 713 0.198 713 0.198 713 0.198 713 0.198 713 0.198 713 0.198 713 0.198 4 0.197 8 0.196 3 0.192 4 0.187 5 0.156 3 0.130 7 0.107 7  Ans.  true log  0 0 0.000 2 5032.388 -3.699 01 0.000 3 10 064.78 -3.522 94 0.000 5 15 097.17 -3.301 14 0.000 65 20 129.55 -3.187 23 0.001 149 35 226.72 -2.939 55 0.001 399 42 272.06 -2.854 18 0.001 575 44 354.84 -2.802 61 0.004 604 46 511.63 -2.336 85 0.012 216 46 357.62 -1.913 05 0.032 284 68 607.07 -1.491 01 0.058 082 81 066.67 -1.235 96 0.240 083 108 765.20 -0.619 64 0.418 956 125 478.20 -0.377 83 0.612 511 137 418.80 -0.212 89 log  true 3.701 774 4.002 804 4.178 895 4.303 834 4.546 872 4.626 053 4.646 941 4.667 562 4.666 121 4.836 369 4.908 842 5.036 49 5.098 568 5.138 046 Chapter 2 - Rev. D, Page 5/19
6. 6. ______________________________________________________________________________ 2-8 Tangent modulus at  = 0 is E  5000  0   25 106 psi 3  0.2 10  0     Ans. At  = 20 kpsi Chapter 2 - Rev. D, Page 6/19
7. 7.  26  19  103  E20   14.0 106  3 1.5  1 10  Ans. psi  (10-3)  (kpsi) 0 0 0.20 5 0.44 10 0.80 16 1.0 19 1.5 26 2.0 32 2.8 40 3.4 46 4.0 49 5.0 54 ______________________________________________________________________________ 2-9 W = 0.20, (a) Before cold working: Annealed AISI 1018 steel. Table A-22, S y = 32 kpsi, S u = 49.5 kpsi,  0 = 90.0 kpsi, m = 0.25,  f = 1.05 After cold working: Eq. (2-16),  u = m = 0.25 A0 1 1 Eq. (2-14),    1.25 Ai 1  W 1  0.20 A Eq. (2-17),  i  ln 0  ln1.25  0.223   u Ai Eq. (2-18), S y   0 im  90  0.223 Eq. (2-19), Su  (b) Before: Su 49.5   1.55 32 Sy 0.25  61.8 kpsi Su 49.5   61.9 kpsi 1  W 1  0.20 After: Ans. 93% increase Ans. 25% increase Su 61.9   1.00 S y 61.8 Ans. Ans. Ans. Lost most of its ductility ______________________________________________________________________________ 2-10 W = 0.20, (a) Before cold working: AISI 1212 HR steel. Table A-22, S y = 28 kpsi, S u = 61.5 kpsi,  0 = 110 kpsi, m = 0.24,  f = 0.85 After cold working: Eq. (2-16),  u = m = 0.24 Chapter 2 - Rev. D, Page 7/19
8. 8. Eq. (2-14), Eq. (2-17), A0 1 1    1.25 Ai 1  W 1  0.20 A  i  ln 0  ln1.25  0.223   u Ai Eq. (2-18), S y   0 im  110  0.223 Eq. (2-19), Su  (b) Before: Su 61.5   2.20 28 Sy 0.24  76.7 kpsi Su 61.5   76.9 kpsi 1  W 1  0.20 After: Ans. 174% increase Ans. 25% increase Su 76.9   1.00 S y 76.7 Ans. Ans. Ans. Lost most of its ductility ______________________________________________________________________________ 2-11 W = 0.20, (a) Before cold working: 2024-T4 aluminum alloy. Table A-22, S y = 43.0 kpsi, S u = 64.8 kpsi,  0 = 100 kpsi, m = 0.15,  f = 0.18 After cold working: Eq. (2-16),  u = m = 0.15 A0 1 1 Eq. (2-14),    1.25 Ai 1  W 1  0.20 A Eq. (2-17), Ans.  i  ln 0  ln1.25  0.223   f Material fractures. Ai ______________________________________________________________________________ 2-12 For H B = 275, Eq. (2-21), S u = 3.4(275) = 935 MPa Ans. ______________________________________________________________________________ 2-13 Gray cast iron, H B = 200. Eq. (2-22), S u = 0.23(200)  12.5 = 33.5 kpsi Ans. From Table A-24, this is probably ASTM No. 30 Gray cast iron Ans. ______________________________________________________________________________ Ans. 2-14 Eq. (2-21), 0.5H B = 100  H B = 200 ______________________________________________________________________________ Chapter 2 - Rev. D, Page 8/19
9. 9. 2-15 For the data given, converting H B to S u using Eq. (2-21) S u (kpsi) 115 116 116 117 117.5 117.5 117.5 118 118 119.5 HB 230 232 232 234 235 235 235 236 236 239 S u = 1172 Su  S N u  S u 2 (kpsi) 13225 13456 13456 13689 13806.25 13806.25 13806.25 13924 13924 14280.25 S u 2 = 137373 1172  117.2  117 kpsi Ans. 10 Eq. (20-8), 10 S 2 u  NSu2 137373  10 117.2  s Su    1.27 kpsi Ans. N 1 9 ______________________________________________________________________________ i 1 2 2-16 For the data given, converting H B to S u using Eq. (2-22) HB 230 232 232 234 235 235 235 236 236 239 S u (kpsi) 40.4 40.86 40.86 41.32 41.55 41.55 41.55 41.78 41.78 42.47 S u = 414.12 S u 2 (kpsi) 1632.16 1669.54 1669.54 1707.342 1726.403 1726.403 1726.403 1745.568 1745.568 1803.701 S u 2 = 17152.63 Chapter 2 - Rev. D, Page 9/19
10. 10. Su  S u N  414.12  41.4 kpsi Ans. 10 Eq. (20-8), 10 S 2 u  NSu2 17152.63  10  41.4   1.20 Ans. N 1 9 ______________________________________________________________________________ s Su  i 1 uR  2-17 (a) 2  45.52  34.5 in  lbf / in 3 2(30) Ans. (b) P L 0 1000 2000 3000 4000 7000 8400 8800 9200 9100 13200 15200 17000 16400 14800 A0 / A – 1   = P/A 0 0.012 291 0.032 811 0.059 802 0.271 355 0.520 373 0.845 059 0 0.0002 0.0003 0.0005 0.000 65 0.001 15 0.0014 0.0018 0.004 45 0.012 291 0.032 811 0.059 802 0.271 355 0.520 373 0.845 059 0 5 032.39 10 064.78 15 097.17 20 129.55 35 226.72 42 272.06 44 285.02 46 297.97 45 794.73 66 427.53 76 492.30 85 550.60 82 531.17 74 479.35 0 0.0004 0.0006 0.0010 0.0013 0.0023 0.0028 0.0036 0.0089 A 0.1963 0.1924 0.1875 0.1563 0.1307 0.1077 From the figures on the next page, 5 1 uT   Ai  (43 000)(0.001 5)  45 000(0.004 45  0.001 5) 2 i 1 1   45 000  76 500  (0.059 8  0.004 45) 2 81 000  0.4  0.059 8  80 000  0.845  0.4    66.7 103 in  lbf/in 3 Ans. Chapter 2 - Rev. D, Page 10/19
11. 11. Chapter 2 - Rev. D, Page 11/19
12. 12. These problems are for student research. No standard solutions are provided. 2-18, 2-19 ______________________________________________________________________________ 2-20 Appropriate tables: Young’s modulus and Density (Table A-5)1020 HR and CD (Table A20), 1040 and 4140 (Table A-21), Aluminum (Table A-24), Titanium (Table A-24c) Appropriate equations: F F For diameter,     Sy A  / 4  d 2  d 4F    Sy Weight/length = A, Cost/length = \$/in = (\$/lbf) Weight/length, Deflection/length =  /L = F/(AE) With F = 100 kips = 100(103) lbf, Young's  Yield  Weight/  Cost/  Deflection/  Material  Modulus  Density   Strength  Cost/lbf Diameter length  length  length  units  Mpsi  lbf/in^3  kpsi  \$/lbf  in  lbf/in  \$/in  in/in                      1020 HR  30  0.282  30 \$0.27 2.060 0.9400 \$0.25  1.000E‐03 1020 CD  30  0.282  57 \$0.30 1.495 0.4947 \$0.15  1.900E‐03 1040  30  0.282  80 \$0.35 1.262 0.3525 \$0.12  2.667E‐03 4140  30  0.282  165 \$0.80 0.878 0.1709 \$0.14  5.500E‐03 Al  10.4  0.098  50 \$1.10 1.596 0.1960 \$0.22  4.808E‐03 Ti  16.5  0.16  120 \$7.00 1.030 0.1333 \$0.93  7.273E‐03 The selected materials with minimum values are shaded in the table above. Ans. ______________________________________________________________________________ 2-21 First, try to find the broad category of material (such as in Table A-5). Visual, magnetic, and scratch tests are fast and inexpensive, so should all be done. Results from these three would favor steel, cast iron, or maybe a less common ferrous material. The expectation would likely be hot-rolled steel. If it is desired to confirm this, either a weight or bending test could be done to check density or modulus of elasticity. The weight test is faster. From the measured weight of 7.95 lbf, the unit weight is determined to be w W 7.95 lbf   0.281 lbf/in 3  0.28 lbf/in3 2 Al [ (1 in) / 4](36 in) which agrees well with the unit weight of 0.282 lbf/in3 reported in Table A-5 for carbon steel. Nickel steel and stainless steel have similar unit weights, but surface finish and darker coloring do not favor their selection. To select a likely specification from Table Chapter 2 - Rev. D, Page 12/19
13. 13. A-20, perform a Brinell hardness test, then use Eq. (2-21) to estimate an ultimate strength of Su  0.5H B  0.5(200)  100 kpsi . Assuming the material is hot-rolled due to the rough surface finish, appropriate choices from Table A-20 would be one of the higher carbon steels, such as hot-rolled AISI 1050, 1060, or 1080. Ans. ______________________________________________________________________________ 2-22 First, try to find the broad category of material (such as in Table A-5). Visual, magnetic, and scratch tests are fast and inexpensive, so should all be done. Results from these three favor a softer, non-ferrous material like aluminum. If it is desired to confirm this, either a weight or bending test could be done to check density or modulus of elasticity. The weight test is faster. From the measured weight of 2.90 lbf, the unit weight is determined to be W 2.9 lbf w   0.103 lbf/in 3  0.10 lbf/in 3 Al [ (1 in)2 / 4](36 in) which agrees reasonably well with the unit weight of 0.098 lbf/in3 reported in Table A-5 for aluminum. No other materials come close to this unit weight, so the material is likely aluminum. Ans. ______________________________________________________________________________ 2-23 First, try to find the broad category of material (such as in Table A-5). Visual, magnetic, and scratch tests are fast and inexpensive, so should all be done. Results from these three favor a softer, non-ferrous copper-based material such as copper, brass, or bronze. To further distinguish the material, either a weight or bending test could be done to check density or modulus of elasticity. The weight test is faster. From the measured weight of 9 lbf, the unit weight is determined to be w W 9.0 lbf   0.318 lbf/in 3  0.32 lbf/in 3 2 Al [ (1 in) / 4](36 in) which agrees reasonably well with the unit weight of 0.322 lbf/in3 reported in Table A-5 for copper. Brass is not far off (0.309 lbf/in3), so the deflection test could be used to gain additional insight. From the measured deflection and utilizing the deflection equation for an end-loaded cantilever beam from Table A-9, Young’s modulus is determined to be 100  24  Fl 3   17.7 Mpsi E 3Iy 3  (1) 4 64  (17 / 32) 3 which agrees better with the modulus for copper (17.2 Mpsi) than with brass (15.4 Mpsi). The conclusion is that the material is likely copper. Ans. ______________________________________________________________________________ 2-24 and 2-25 These problems are for student research. No standard solutions are provided. ______________________________________________________________________________ Chapter 2 - Rev. D, Page 13/19
14. 14. 2-26 For strength,  = F/A = S  A = F/S For mass, m = Al = (F/S) l Thus, f 3 (M ) =  /S , and maximize S/ ( = 1) In Fig. (2-19), draw lines parallel to S/ From the list of materials given, both aluminum alloy and high carbon heat treated steel are good candidates, having greater potential than tungsten carbide or polycarbonate. The higher strength aluminum alloys have a slightly greater potential. Other factors, such as cost or availability, may dictate which to choose. Ans. ______________________________________________________________________________ 2-27 For stiffness, k = AE/l  A = kl/E For mass, m = Al = (kl/E) l =kl2  /E Thus, f 3 (M) =  /E , and maximize E/ ( = 1) In Fig. (2-16), draw lines parallel to E/ Chapter 2 - Rev. D, Page 14/19
15. 15. From the list of materials given, tungsten carbide (WC) is best, closely followed by aluminum alloys, and then followed by high carbon heat-treated steel. They are close enough that other factors, like cost or availability, would likely dictate the best choice. Polycarbonate polymer is clearly not a good choice compared to the other candidate materials. Ans. ______________________________________________________________________________ 2-28 For strength,  = Fl/Z = S (1) where Fl is the bending moment and Z is the section modulus [see Eq. (3-26b), p. 90 ]. The section modulus is strictly a function of the dimensions of the cross section and has the units in3 (ips) or m3 (SI). Thus, for a given cross section, Z =C (A)3/2, where C is a  number. For example, for a circular cross section, C = 4   1 . Then, for strength, Eq. (1) is Fl S CA3/2   Fl  A   CS  2/3 (2) Chapter 2 - Rev. D, Page 15/19
16. 16. For mass, Thus,  Fl  m  Al      CS  2/3 F l    C 2/3    l 5/3  2/3  S  f 3 (M) =  /S 2/3, and maximize S 2/3/ ( = 2/3) In Fig. (2-19), draw lines parallel to S 2/3/ From the list of materials given, a higher strength aluminum alloy has the greatest potential, followed closely by high carbon heat-treated steel. Tungsten carbide is clearly not a good choice compared to the other candidate materials. .Ans. ______________________________________________________________________________ 2-29 Eq. (2-26), p. 65, applies to a circular cross section. However, for any cross section shape it can be shown that I = CA 2, where C is a constant. For example, consider a rectangular section of height h and width b, where for a given scaled shape, h = cb, where c is a Chapter 2 - Rev. D, Page 16/19
17. 17. constant. The moment of inertia is I = bh 3/12, and the area is A = bh. Then I = h(bh2)/12 = cb (bh2)/12 = (c/12)(bh)2 = CA 2, where C = c/12 (a constant). Thus, Eq. (2-27) becomes 1/2  kl 3  A   3CE  and Eq. (2-29) becomes  k  5/2    m  Al     l  1/2   3C  E  1/2 Thus, minimize f3  M    E 1/ 2 , or maximize M  E1/2  . From Fig. (2-16) From the list of materials given, aluminum alloys are clearly the best followed by steels and tungsten carbide. Polycarbonate polymer is not a good choice compared to the other candidate materials. Ans. ______________________________________________________________________________ 2-30 For stiffness, k = AE/l  A = kl/E For mass, m = Al = (kl/E) l =kl2  /E Chapter 2 - Rev. D, Page 17/19
18. 18. So, f 3 (M) =  /E, and maximize E/ . Thus,  = 1. Ans. ______________________________________________________________________________ 2-31 For strength,  = F/A = S  A = F/S For mass, m = Al = (F/S) l So, f 3 (M ) =  /S, and maximize S/ . Thus,  = 1. Ans. ______________________________________________________________________________ 2-32 Eq. (2-26), p. 65, applies to a circular cross section. However, for any cross section shape it can be shown that I = CA 2, where C is a constant. For example, consider a rectangular section of height h and width b, where for a given scaled shape, h = cb, where c is a constant. The moment of inertia is I = bh 3/12, and the area is A = bh. Then I = h(bh2)/12 = cb (bh2)/12 = (c/12)(bh)2 = CA 2, where C = c/12. Thus, Eq. (2-27) becomes 1/2  kl 3  A   3CE  and Eq. (2-29) becomes  k  5/2    m  Al     l  1/2   3C  E  1/2 So, minimize f3  M    E1/2 , or maximize M  . Thus,  = 1/2. Ans.  E 1/ 2 ______________________________________________________________________________ 2-33 For strength,  = Fl/Z = S (1) where Fl is the bending moment and Z is the section modulus [see Eq. (3-26b), p. 90 ]. The section modulus is strictly a function of the dimensions of the cross section and has the units in3 (ips) or m3 (SI). Thus, for a given cross section, Z =C (A)3/2, where C is a  number. For example, for a circular cross section, C = 4   1 . Then, for strength, Eq. (1) is Fl S CA3/2 For mass,  Fl  A   CS    Fl  m  Al      CS  2/3 F l    C 2/3 2/3 (2)    l 5/3  2/3  S  So, f 3 (M) =  /S 2/3, and maximize S 2/3/. Thus,  = 2/3. Ans. ______________________________________________________________________________ 2-34 For stiffness, k=AE/l, or, A = kl/E. Chapter 2 - Rev. D, Page 18/19
19. 19. Thus, m = Al = (kl/E )l = kl 2  /E. Then, M = E / and  = 1. From Fig. 2-16, lines parallel to E / for ductile materials include steel, titanium, molybdenum, aluminum alloys, and composites. For strength, S = F/A, or, A = F/S. Thus, m = Al = F/Sl = Fl  /S. Then, M = S/ and  = 1. From Fig. 2-19, lines parallel to S/ give for ductile materials, steel, aluminum alloys, nickel alloys, titanium, and composites. Common to both stiffness and strength are steel, titanium, aluminum alloys, and composites. Ans. Chapter 2 - Rev. D, Page 19/19